HAL Id: hal-01166423
Submitted on 26 Sep 2015
HAL is a multi-disciplinary open access
archive for the deposit and dissemination of
sci-entific research documents, whether they are
pub-lished or not. The documents may come from
teaching and research institutions in France or
abroad, or from public or private research centers.
L’archive ouverte pluridisciplinaire HAL, est
destinée au dépôt et à la diffusion de documents
scientifiques de niveau recherche, publiés ou non,
émanant des établissements d’enseignement et de
recherche français ou étrangers, des laboratoires
publics ou privés.
Radiative Thermal Rectification between SiC and SiO2
Karl Joulain, Younes Ezzahri, Jérémie Drevillon, Benoit Rousseau, Domingos
de Sousa Meneses
To cite this version:
Karl Joulain, Younes Ezzahri, Jérémie Drevillon, Benoit Rousseau, Domingos de Sousa Meneses.
Radiative Thermal Rectification between SiC and SiO2. Optics Express, Optical Society of America
- OSA Publishing, 2015, 23 (24), pp.A1388-A1397. �10.1364/OE.23.0A1388�. �hal-01166423v2�
Radiative thermal rectification between
SiC and SiO
Karl Joulain,1,∗Youn`es Ezzahri,1J´er´emie Drevillon,1Benoˆıt Rousseau,2and Domingos De Sousa Meneses,3,∗
1Institut Pprime, Universit´e de Poitiers-CNRS-ENSMA, TSA 41105, F-86073 Poitiers, France 2LTN, CNRS UMR 6607, B.P 90604, F-44306 Nantes, France
3CNRS, CEMHTI UPR3079, Universit´e d’Orl´eans, F-45071 Orl´eans, France ∗email@example.com, firstname.lastname@example.org
Abstract: By means of fluctuational electrodynamics, we calculate radiative heat flux between two planar materials respectively made of SiC and SiO2. More specifically, we focus on a first (direct) situation where one of the two materials (for example SiC) is at ambient temperature whereas the second material is at a higher one, then we study a second (reverse) situation where the material temperatures are inverted. When the two fluxes corresponding to the two situations are different, the materials are said to exhibit thermal rectification, a property with potential applications in thermal regulation. Rectification variations with temperature and separation distance are reported here. Calculations are performed using material optical data experimentally determined by Fourier transform emission spectrometry of heated materials between ambient temperature (around 300 K) and 1480 K. It is shown that rectification is much more important in the near-field domain, i.e. at separation distances smaller than the thermal wavelength. In addition, we see that the larger is the temperature difference, the larger is rectification. Large rectification is finally interpreted due to a weakening of the SiC surface polariton when temperature increases, a weakening which affects much less SiO2resonances.
© 2015 Optical Society of America
OCIS codes: (160.6840) Thermo-optical materials; (260.2160) Energy transfer; (290.6815) Thermal emission; (350.5610) Radiation
References and links
1. S.M. Rytov, Principle of Statistical Radiophysics 3. Elements of Radiation Fields (Springer Verlag, 1989). 2. D. Polder and M. van Hove, “Theory of radiative heat transfer between closely spaced bodies ,” Phys. Rev. B 4,
3. J. P. Mulet, K. Joulain, R. Carminati, and J. J. Greffet, “Enhanced radiative heat transfer at nanometric distances,” Microscale Thermophysical Engineering 6, 209–222 (2002).
4. P. Ben-Abdallah and K. Joulain, “Fundamental limits for noncontact transfers between two bodies,” Phys. Rev. B 82, 121419(R) (2010).
5. E. Nefzaoui, Y. Ezzahri, J. Drevillon, and K. Joulain, “Maximal near-field radiative heat transfer between two plates,” The European Physical Journal Applied Physics 63, 30902 (2013).
6. J.M. Ziman, Electrons and Phonons (Oxford University Press, 1960).
7. M. Terraneo, M. Peyrard, and G. Casati, “Controlling the energy flow in nonlinear lattices: a model for a thermal rectifier ,” Phys. Rev. Lett. 88, 094302 (2002).
8. B. Li, L. Wang, and G. Casati, “Thermal diode : rectification of heat flux,” Phys. Rev. Lett. 93, 184301 (2004). 9. B. Li, J. Lan, and L. Wang, “Interface thermal resistance between dissimilar anharmonic lattices ,” Phys. Rev.
10. C. W. Chang, D. Okawa, A. Majumdar, and A. Zettl, “Solid-state thermal rectifier,” Science 314, 1121–1124 (2006).
11. B. Hu, L. Yang, and Y. Zhang, “Asymmetric heat conduction in nonlinear lattices,” Phys. Rev. Lett. 97, 124302 (2006).
12. J. Hu, X. Ruan, and Y. P. Chen, “Thermal conductivity and thermal rectification in graphene nanoribbons: a molecular dynamics study,” Nano Letters 9, 2730–2735 (2009).
13. N. Yang, N. Li, L. Wang, and B. Li, “Thermal rectification and negative differential thermal resistance in lattices with mass gradient ,” Phys. Rev. B 76, 020301(R) (2007).
14. D. Segal, “Single mode heat rectifier: controlling energy flow between electronic conductors ,” Phys. Rev. Lett. 100, 105901 (2008).
15. N. Yang, G. Zhang, and B. Li, “Thermal rectification in asymmetric graphene ribbons,” Appl. Phys. Lett. 95, 033107 (2009).
16. L. Wang and B. Li, “Thermal logic gates: computation with phonons ,” Phys. Rev. Lett. 99, 177208 (2007). 17. W. C. Lo, L. Wang, and B. Li, “Thermal transistor: heat flux switching and modulating,” Journal of the Physical
Society of Japan 77, 054402 (2008).
18. C. R. Otey, W. T. Lau, and S. Fan, “Thermal rectification through vacuum,” Phys. Rev. Lett. 104, 154301 (2010). 19. S. Basu and M. Francoeur, “Near-field radiative transfer based thermal rectification using doped silicon ,” Appl.
Phys. Lett. 98, 113106 (2011).
20. P. Ben-Abdallah and S.-A. Biehs, “Phase-change radiative thermal diode,” Appl. Phys. Lett. 103, 191907 (2013). 21. E. Nefzaoui, J. Drevillon, Y. Ezzahri, and K. Joulain, “Simple far-field radiative thermal rectifier using Fabry–
Perot cavities based infrared selective emitters,” Appl. Opt. 53, 3479 (2014).
22. E. Nefzaoui, K. Joulain, J. Drevillon, and Y. Ezzahri, “Radiative thermal rectification using superconducting materials,” Appl. Phys. Lett. 104, 103905 (2014).
23. P. Ben-Abdallah and S.-A. Biehs, “Near-field thermal transistor,” Phys. Rev. Lett. 112, 044301 (2014). 24. K. Joulain, Y. Ezzahri, J. Drevillon, and P. Ben-Abdallah, “Modulation and amplification of radiative far field
heat transfer:Towards a simple radiative thermal transistor,” Appl. Phys. Lett. 106, 133505 (2015).
25. P. van Zwol, L. Ranno, and J. Chevrier, “Emissivity measurements with an atomic force microscope ,” J. Appl. Phys. 111, 063110 (2012).
26. J. Huang, Q. Li, Z. Zheng, and Y. Xuan, “Thermal rectification based on thermochromic materials ,” International Journal of Heat and Mass Transfer 67, 575–580 (2013).
27. H. Iizuka and S. Fan, “Rectification of evanescent heat transfer between dielectric-coated and uncoated silicon carbide plates,” J. Appl. Phys. 112, 024304 (2012).
28. D. Olego and M. Cardona, “Temperature dependence of the optical phonons and transverse effective charge in 3C-SiC,” Phys. Rev. B 25, 3889 (1982).
29. D. De Sousa Meneses, P. Melin, L. del Campo, L. Cosson, and P. Echegut, “Infrared Physics & Technology,” Infrared Physics & Technology 69, 96–101 (2015).
30. D. De Sousa Meneses, J.-F. Brun, P. Echegut, and P. Simon, “Contribution of Semi-Quantum Dielectric Function Models to the Analysis of Infrared Spectra,” Applied Spectroscopy pp. 1–6 (2004).
31. D. De Sousa Meneses, M. Malki, and P. Echegut, “Optical and structural properties of calcium silicate glasses,” Journal of Non-Crystalline Solids 352, 5301–5308 (2006).
32. D. De Sousa Meneses, M. Eckes, L. del Campo and P. Echegut, “Phase transformations of crystalline SiO2versus
dynamic disorder between room temperature and liquid state,” Journal of Physics: Condensed Matter 26, 255402 (2014).
33. S. A. Biehs, E. Rousseau, and J. J. Greffet, “Mesoscopic description of radiative heat transfer at the nanoscale,” Phys. Rev. Lett. 105, 234301 (2010).
34. P.-O. Chapuis, S. Volz, C. Henkel, K. Joulain, and J.-J. Greffet, “Effects of spatial dispersion in near-field radiative heat transfer between two parallel metallic surfaces,” Phys. Rev. B 77, 035431 (2008).
35. F. Singer, Y. Ezzahri, and K. Joulain, “Near field radiative heat transfer between two nonlocal dielectrics,” J. Quant. Spectr. and Rad. Transf. 154, 55–62 (2015).
36. K. Joulain, J.-P. Mulet, F. Marquier, R. Carminati, and J.-J. Greffet, “Surface electromagnetic waves thermally excited: Radiative heat transfer, coherence properties and Casimir forces revisited in the near field,” Surf. Sci. Rep. 57, 59–112 (2005).
37. A. Volokitin and B. Persson, “Near-field radiative heat transfer and noncontact friction,” Rev. Mod. Phys. 79, 1291–1329 (2007).
38. E. Rousseau, M. Laroche, and J.-J. Greffet, “Asymptotic expressions describing radiative heat transfer between polar materials from the far-field regime to the nanoscale regime,” J. Appl. Phys. 111, 014311 (2012). 39. K. Ito, K. Nishikawa, H. Izuka and H. Toshiyoshi, “Experimental investigation of radiative thermal rectifier using
Since the seminal works of Rytov  and Polder and Van Hove , it has been known that radiative heat transfer (RHT) can be much larger than classical Planck’s prediction when the separation distance between two solid bodies are small compared to the thermal wavelength at which heat radiation is exchanged. Enhancement is particularly large in the case of dielectrics supporting phonon-polariton such as SiC or SiO2 that have probably been the most stud-ied materials in the framework of near-field heat transfer. In the case of materials supporting polaritons, these non radiative modes can couple so that heat is transferred in vacuum through photon tunneling. However, the magnitude of the enhancement strongly depends on the ampli-tude and the width of the resonance in the material optical response which can be affected by its temperature [4, 5]. Indeed, when the temperature increases, one knows that phonons in general including phonon-polaritons are affected by several processes like phonon-phonon interactions so that theses modes see their lifetime decreases . But phonons in different materials are not equally affected by temperature changes.
A question which naturally arises is whether the heat flux between a material at ambient tem-perature and another one different at a higher temtem-perature will be the same when temtem-peratures are inverted. If it is not the case, the two materials couple is said to exhibit thermal rectification, a thermal analog of electrical rectification better known as the diode.
Thermal rectification has recently received a growing interest due to the emergence of ther-mal flow management needs related to limited energy and global warming issues. If therther-mal equivalent of the diode and the transistor would be designed and fabricated, this could open the way to new passive temperature regulation and thermal circuits with no needs of electronics leading to very reliable thermal management.
In the last decade, thermal conductors exhibiting thermal rectification have been proposed. In these devices, heat carriers flux is made asymmetric by nanostructuring the material or by guid-ing the carriers flux differently whether they are movguid-ing in one direction or the other [7–15]. These physical ideas can be used to conceive and fabricate a thermal transistor leading to the possibility of logical thermal circuits [16, 17]. More recently, radiative thermal rectifiers have been proposed [18–22] as well as radiative thermal transistors [23, 24]. Very promising devices have been imagined based on materials exhibiting phase change transition such as Vanadium dioxyde (VO2) [20, 23, 25], superconductors  or thermochromic materials . The goal of this article is to show that radiative thermal rectification can also be achieved with the most studied polaritonic supported materials like SiC and SiO2.
We first present optical properties measurements showing how both SiC and SiO2dielectric functions change with temperature. These measurements performed using Fourier Transform Emission Spectroscopy allow us to make near-field radiative heat transfer calculations taking into account the actual material dependance with temperature. Similar near-field calculation taking into account the temperature dependance of optical properties have already been taken in the past  with measurement on 3-C SiC of  but in a different situation between SiC and metallic coated-SiC. Here, we calculate heat transfer between two planar interfaces of SiC and SiO2. We show that these two materials exhibit almost no thermal rectification when the exchange occurs in the far-field i.e. when the main contribution to the flux comes from the propagative waves. On the contrary, at distances below 100 nm, we show that rectification ratio drastically increases in order to reach values as high as the highest predicted and measured ones in the literature. We finally show that rectification is mainly due to the SiC resonance attenuation at high temperature.
2. SiC and SiO2optical datas
In this section, we report SiC and SiO2optical properties temperature dependance with tem-perature. The dielectric functions of SiC and vitreous SiO2have been extracted from measure-ments of their spectral emittance at near normal incidence. The SiC sample provided by MTI Corporation is a single crystal with a (0001) orientation and two epi polished sides. The stacking sequence is of 6H type and its electric resistivity lies between 0.02 and 0.2 ohm.cm. The SiO2 material is a polished plate of vitreous silica with low OH content (< 20ppm). The emittance spectra were acquired with a homemade spectrometer built around two Bruker infrared spec-trometers, a Vertex 80v working under vacuum and a Vertex 70 purged with dry air (see ). The first and second devices have been used to probe the far- and mid-infrared ranges respec-tively, at a spectral resolution of 4 cm−1. In order to avoid parasite fluxes during the measure-ments, a CO2laser has been used to heat the samples up to 1500 K. The retrieval of the optical functions has been performed in a second step by fitting the experimental data with adequate physical expressions. A semi-quantum dielectric function model, well adapted for crystalline media, was selected to reproduce the infrared response of the silicon carbide sample . The disordered nature of vitreous silica needed instead the use of a causal Gaussian dielectric func-tion model able to take account for the inhomogeneous broadening of the absorpfunc-tion bands of glasses . The whole process allowed to obtain the temperature dependences of the opti-cal properties for both materials in a wide range, the results are reported in Fig. 1. For SiO2, we note that the resonance around 2×1014rad s−1slightly shifts and broadens when the tem-perature increases. For SiC, we note a similar behavior (shift and broadening) but even more pronounced for the resonance around 1.5×1014rad s−1. This is due to the fact that anharmonic-ity effects responsible of the phonon-phonon interaction increases with the temperature . We will see that this behavior is responsible for the important rectification between SiO2and SiC in the near-field. Note however that the second resonance in SiO2does not change a lot with temperature as long as temperature is below the vitreous transition which occur around 1500 K . This is probably related to the very weak SiO2thermal dilatation.
3. Radiative heat transfer between SiC and SiO2
We now come to the calculation of the RHT between two planar interfaces made of SiC (medium 1) and SiO2 (medium2). RHT between two planar interfaces can easily be calcu-lated using fluctuational electrodynamics formalism. Heat flux appears as a semi-analytical expressions which is nothing else than the summation of individual plane wave contributions to the heat transfer. These plane waves are labelled by a triplet(ω, K,α) whereω is the angular frequency of the wave, K is the wavector component parallel to the interfaces whereas α is the wave polarization (s or p). Let us call T1temperature of medium 1 and T2temperature of medium 2. Heat flux expression between media 1 and 2 reads [4, 33]
∑α=s,p Z ∞ 0 [Θ( ω, T1) − Θ(ω, T2)]dω Z ∞ 0 KdK 4π2 τ α(ω, K) (1)
where Θ(ω, T ) = ¯hω/[exp[¯hω/kbT] − 1] is the mean energy of a photon at temperature T . In the preceding expression,τα(ω, K) appears as a transmission coefficient for a plane wave (ω, K,α) between medium 1 and medium 2 or medium 2 and medium 1. Note that expres-sions of transmission coefficient are different whether the wave is propagative (K<ω/c or evanescent (K>ω/c). If we call medium 3, the medium separating the two other media and introducing Fresnel reflection coefficients, the expression for the transmission coefficient reads for propagating waves
τα(ω, K) =(1 − |r α 31|2)(1 − |r32α|2) |1 − rα 31rα32e2iγ3d|2 (2)
Fig. 1. Measured real and Imaginary part of the dielectric functionε variation with angular frequencyω for different temperatures. Top 2 figures : SiO2. Bottom 2 figures : SiC.
and for evanescent waves τα(ω, K) =4ℑ(r α 31)ℑ(rα32)e−2ℑ(γ3)d |1 − rα 31rα32e−2ℑ(γ3)d|2 (3)
In these expressions,ℑ denotes the imaginary part,γiis the perpendicular wave vector compo-nent in medium i which for non magnetic materials readsγi= (εik20− K2)1/2. The usual fresnel reflection coefficient are given by rs
i j= (γi−γj)/(γi+γj) and ri jp = (εjγi−εiγj)/(εjγi+εiγj) when one considers local materials which is the case at nanometric separation distance [34,35]. The flux expression only depends on the material temperatures, their local optical response and the separation distance between the bodies. Note that the symmetry of Eq. (1) implies that recti-fication will occur if and only if the two materials are different and have their optical properties that change with temperature in a different manner.
Optical properties variations with temperature have rarely been taken into account, mostly in the case of phase change materials. Here, our main goal is to perform these calculations in the case of two very well studied materials but for which optical properties variations with tem-perature are taken into account. The input properties in our calculation are the optical properties presented in the preceding section. It can be noted in these measurements that they have been taken at close temperatures for both materials but not exactly at the same one. As explained in the introduction, our goal is also to explore how a system constituted of SiC and SiO2can exhibit radiative thermal rectification. Thus, a difficulty arises since rectification compares a situation where the materials are at two different temperatures with a second situation where the temperatures considered before have been inverted. For example, measurements at ambient temperature for SiC have been performed at 295 K whereas they have been performed at 298 K for SiO2. In our calculation, we choosed ambient temperature to be 297 K and we assumed that optical properties at this temperature were the ones at 295 K for SiC and 298K for SiO2. Other temperatures considered in the paper are 471 K, 671 K, 981 K, 1102 K and 1470 K. To perform heat flux calculations, optical properties for SiC and SiO2have been respectively taken at 464 K and 479 K, 686 K and 672 K, 996 K and 966 K, 1105 K and 1098 K, 1460 K and 1480 K (See Fig. 1).
We report in Fig. 2 heat flux variations as a function of the separation distance between the two materials. We compare the situation where SiO2is at 297 K and SiC at 1470 K with the situation where the temperatures are inverted. We note that for separation distances larger than a few microns the two fluxes are constant and almost superimposed each other. When SiO2is at ambient temperature, the value of the heat flux is 1.872×105W m−2whereas it is 1.896×105W m−2in the reverse case. These two values are around 71% of the heat exchanged between two blackbodies for which Fresnel reflection factors are equal to 0 in the fluxes expression. When the separation distance is decreased, the heat flux increases for both situations. For distances larger than 200 nm, heat fluxes are very close in both situations. For distances smaller than 200 nm, we see that the situation where SiC remains at ambient temperature exhibits a higher flux than the one corresponding to the reverse one.
We define rectification R as the relative variation of the heat flux [20,21] in the two situations so that
R= |ϕ1↔2(T1, T2) −ϕ1↔2(T2, T1)| Max[ϕ1↔2(T1, T2),ϕ1↔2(T2, T1)]
With such a definition, R= 0 means the the material exhibit no rectification whereas R = 1 correspond to the case of a perfect thermal diode. In Fig. 3, we report the variation of the rectification as a function of the separation distance between the two planar interfaces made of SiC and SiO2for different temperatures. One material is always at 297 K whereas the second one is taken at 471 K, 671 K, 981 K, 1102 K or 1470 K. We note a very similar behavior for
Fig. 2. Computed radiative heat transfer between a plane interface of SiC and a second one constituted of SiO2versus their separation distances. Two situations are compared. In the
first one (plain) SiO2is at 297 K and SiC at 1470 K whereas in the second one (dashed)
SiC is at 297 K and SiO2is at 1470 K.
Fig. 3. Computed rectification variations as a function of the separation distance between two planar interfaces made of SiC and SiO2when one material is at 297 K and the second
all the cases presented. For distances larger than 200 nm rectification remains very low. It goes from 10−3for the smallest temperature difference to 10−2 for the largest. One can therefore say that SiC and SiO2exhibit very low radiative thermal rectification in the far field and more generally for separation distances larger than 200 nm. Below 200 nm, rectification increases drastically to reach values up to 0.7 for a temperature of 1470 K. Rectification saturates when the separation distance goes below 10 nm. Note also that the higher temperature difference is, the higher is the rectification in the near-field.
Let us now shed some light on the physical reason that is responsible of the behavior of the rectification between SiC and SiO2 with both distance and temperature. To do so, we plot in Fig. 4 the variation of the spectral radiative heat transfer flux as a function of the angular frequency for the case where one material is at 297 K and the other one at 1470 K. The spectral flux is represented for 4 different separation distances 1 µm, 100 nm, 10 nm and 1nm. At large distance (here 1 µm), the spectral flux is very similar to the one representative of the exchange between two black bodies except that there exist some frequencies where one can identify dips. These dips correspond to the frequencies where SiO2and SiC exhibit resonances. Indeed, SiO2 exhibit two resonances and SiC one resonance that had been identified in the first section. At these frequencies SiO2and SiC are very reflective so that transfer is greatly reduced. However, the range of frequencies where materials are low absorbent is much smaller than the one where both materials almost behave as blackbodies. This explains why at large distance when this spectral flux is integrated over all frequencies, heat flux reaches 70% of the one between two blackbodies. If we examine carefully the region where the spectral flux is much lower than between blackbodies, one see that these are the regions where the spectral fluxes differ in the direct and the reverse situations. We notice that the depth of the dips is less pronounced when the material concerned is at high temperature. For example dips for SiO2 (around 9×1013 rad s−1 and 2× 1014 rad s−1) are less pronounced in the plain curve where SiO2 is at high temperature. In the same way, the dip corresponding to the SiC resonance around 1.5× 1014rad s−1is smaller in the dashed curve corresponding to the case where SiC is at high temperature. Despite of these differences, as most of the contribution comes from the region where the spectral fluxes are equal, rectification in the far-field is very small and even smaller at lower temperature when the dielectric function is still close to the one at ambient temperature.
When the distance is reduced, the situation drastically changes. The main contributions to the spectral fluxes mainly comes from the frequencies where the resonances are present. This is a well known behavior when one is treating materials supporting phonon polaritons such as SiC and SiO2. Indeed, the heat flux is completely dominated by the contribution of evanescent waves in p polarization [36, 37] which depends on the imaginary part of the static reflection coefficient which reads for medium i(εi− 1)/(ε+ 1). The frequency whereεiis approaching -1 corresponds to the one where there is the largest density of states of surface polaritons close to the material. What appears here is that the contribution of the polaritons of a material is reduced when the material is at high temperature. Moreover, one notes that SiO2and SiC do not behave in the same way. While the SiO2resonance contribution is weakly attenuated, the one of SiC is much more decreased by almost one order of magnitude above 1000 K. This explains why the heat flux is larger when the SiC is at low temperature. Moreover rectification does not change below a certain distance which correspond to the one where the flux is completely dominated by the p contribution of the evanescent waves. It has been shown in several papers [3, 36, 38], that this flux behaves as 1/d2multiplied by the product of the imaginary parts of the reflection coefficients. When the distance decreases, both fluxes increase following the same distance
Fig. 4. Computed spectral radiative heat transfer between two planar interfaces made of SiC and SiO2in the direct and the reverse situation for 4 different separation distances:
SiO2is at 297 K and SiC is at 1470 K in the first situation (plain) whereas SiO2is at 1470
scaling law. Therefore, rectification becomes distance independent and saturates.
We have presented in this paper calculation of the radiative heat flux between two materials SiC and SiO2taking into account the real temperature variations of their optical properties. To do so, we have used measurements of the optical response of both SiO2and SiC at different temperatures from the ambient one up to almost 1500K. We show that when the temperature difference between the two samples is large, there is little difference in the far field between the fluxes calculated in a situation where one of the materials is at 297 K and the other one at higher temperature and another situation where the temperatures are reversed. We see that at any temperature difference, rectification increases between 200 nm and 10 nm to reach a value which is crescent with the temperature difference. Using the data measured here, one has shown that this rectification can reach values up to 0.7, values that are as high as the one obtained with phase change materials [20, 39]. These properties could be exploited in thermal management. Thermal radiative rectification could for example be adjusted by controlling the separation distance between the materials and their temperatures.
This work has been supported by CNRS through the grant CARDYMOL of the “Cellule ´energie”. This work also pertains to the French Government Program “Investissement d’Avenir” (LABEX INTERACTIFS, ANR-11-LABX-0017-01).